Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. 5.1 MECHANICAL PROPERTIES OF MATERIALS by John Symonds, Expanded by StaffREFERENCES: Davis et al., ‘‘Testing and Inspection of Engineering Materials,’’ permanent strain. The permanent strain commonly used is 0.20 percentMcGraw-Hill, Timoshenko, ‘‘Strength of Materials,’’ pt . II, Van Nostrand. of the original gage length. The intersection of this line with the curveRichards, ‘‘Engineering Materials Science,’’ Wadsworth. Nadai, ‘‘Plasticity,’’ determines the stress value called the yield strength. In reporting theMcGraw-Hill. Tetelman and McEvily, ‘‘Fracture of Structural Materials,’’ Wiley. yield strength, the amount of permanent set should be speciﬁed. The‘‘Fracture Mechanics,’’ ASTM STP-833. McClintock and Argon (eds.), ‘‘Me- arbitrary yield strength is used especially for those materials not ex-chanical Behavior of Materials,’’ Addison-Wesley. Dieter, ‘‘Mechanical Metal-lurgy,’’ McGraw-Hill. ‘‘Creep Data,’’ ASME. ASTM Standards, ASTM. Blaz- hibiting a natural yield point such as nonferrous metals; but it is notnynski (ed.), ‘‘Plasticity and Modern Metal Forming Technology,’’ Elsevier limited to these. Plastic behavior is somewhat time-dependent, particu-Science. larly at high temperatures. Also at high temperatures, a small amount of time-dependent reversible strain may be detectable, indicative of anelas- tic behavior.STRESS-STRAIN DIAGRAMS The Stress-Strain Curve The engineering tensile stress-strain curveis obtained by static loading of a standard specimen, that is, by applyingthe load slowly enough that all parts of the specimen are in equilibriumat any instant. The curve is usually obtained by controlling the loadingrate in the tensile machine. ASTM Standards require a loading rate notexceeding 100,000 lb/in2 (70 kgf/mm2)/min. An alternate method ofobtaining the curve is to specify the strain rate as the independent vari-able, in which case the loading rate is continuously adjusted to maintainthe required strain rate. A strain rate of 0.05 in/in/(min) is commonlyused. It is measured usually by an extensometer attached to the gagelength of the specimen. Figure 5.1.1 shows several stress-strain curves. Fig. 5.1.2. General stress-strain diagram. The ultimate tensile strength (UTS) is the maximum load sustained by the specimen divided by the original specimen cross-sectional area. The percent elongation at failure is the plastic extension of the specimen at failure expressed as (the change in original gage length ϫ 100) divided by the original gage length. This extension is the sum of the uniform and nonuniform elongations. The uniform elongation is that which occurs prior to the UTS. It has an unequivocal signiﬁcance, being associated with uniaxial stress, whereas the nonuniform elongation which occurs during localized extension (necking) is associated with triaxial stress. The nonuniform elongation will depend on geometry, particularly the ratio of specimen gage length L 0 to diameter D or square root of cross- sectional area A. ASTM Standards specify test-specimen geometry for a number of specimen sizes. The ratio L 0 /√A is maintained at 4.5 for ﬂat- and round-cross-section specimens. The original gage length should always be stated in reporting elongation values. The specimen percent reduction in area (RA) is the contraction in cross-sectional area at the fracture expressed as a percentage of theFig. 5.1.1. Comparative stress-strain diagrams. (1) Soft brass; (2) low carbon original area. It is obtained by measurement of the cross section of thesteel; (3) hard bronze; (4) cold rolled steel; (5) medium carbon steel, annealed; (6) broken specimen at the fracture location. The RA along with the load atmedium carbon steel, heat treated. fracture can be used to obtain the fracture stress, that is, fracture load divided by cross-sectional area at the fracture. See Table 5.1.1. For most engineering materials, the curve will have an initial linear The type of fracture in tension gives some indications of the qualityelastic region (Fig. 5.1.2) in which deformation is reversible and time- of the material, but this is considerably affected by the testing tempera-independent. The slope in this region is Young’s modulus E. The propor- ture, speed of testing, the shape and size of the test piece, and othertional elastic limit (PEL) is the point where the curve starts to deviate conditions. Contraction is greatest in tough and ductile materials andfrom a straight line. The elastic limit (frequently indistinguishable from least in brittle materials. In general, fractures are either of the shear or ofPEL) is the point on the curve beyond which plastic deformation is the separation (loss of cohesion) type. Flat tensile specimens of ductilepresent after release of the load. If the stress is increased further, the metals often show shear failures if the ratio of width to thickness isstress-strain curve departs more and more from the straight line. Un- greater than 6 : 1. A completely shear-type failure may terminate in aloading the specimen at point X (Fig. 5.1.2), the portion XXЈ is linear chisel edge, for a ﬂat specimen, or a point rupture, for a round specimen.and is essentially parallel to the original line OXЈЈ. The horizontal dis- Separation failures occur in brittle materials, such as certain cast irons.tance OXЈ is called the permanent set corresponding to the stress at X. Combinations of both shear and separation failures are common onThis is the basis for the construction of the arbitrary yield strength. To round specimens of ductile metal. Failure often starts at the axis in adetermine the yield strength, a straight line XXЈ is drawn parallel to the necked region and produces a relatively ﬂat area which grows until theinitial elastic line OXЈЈ but displaced from it by an arbitrary value of material shears along a cone-shaped surface at the outside of the speci-5-2
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. STRESS-STRAIN DIAGRAMS 5-3 Table 5.1.1 Typical Mechanical Properties at Room Temperature (Based on ordinary stress-strain values) Tensile Yield Ultimate strength, strength, elongation, Reduction Brinell Metal 1,000 lb/in 2 1,000 lb/in 2 % of area, % no. Cast iron 18 – 60 8 – 40 0 0 100 – 300 Wrought iron 45 – 55 25 – 35 35 – 25 55 – 30 100 Commercially pure iron, annealed 42 19 48 85 70 Hot-rolled 48 30 30 75 90 Cold-rolled 100 95 200 Structural steel, ordinary 50 – 65 30 – 40 40 – 30 120 Low-alloy, high-strength 65 – 90 40 – 80 30 – 15 70 – 40 150 Steel, SAE 1300, annealed 70 40 26 70 150 Quenched, drawn 1,300°F 100 80 24 65 200 Drawn 1,000°F 130 110 20 60 260 Drawn 700°F 200 180 14 45 400 Drawn 400°F 240 210 10 30 480 Steel, SAE 4340, annealed 80 45 25 70 170 Quenched, drawn 1,300°F 130 110 20 60 270 Drawn 1,000°F 190 170 14 50 395 Drawn 700°F 240 215 12 48 480 Drawn 400°F 290 260 10 44 580 Cold-rolled steel, SAE 1112 84 76 18 45 160 Stainless steel, 18-S 85 – 95 30 – 35 60 – 55 75 – 65 145 – 160 Steel castings, heat-treated 60 – 125 30 – 90 33 – 14 65 – 20 120 – 250 Aluminum, pure, rolled 13 – 24 5 – 21 35 – 5 23 – 44 Aluminum-copper alloys, cast 19 – 23 12 – 16 4–0 50 – 80 Wrought , heat-treated 30 – 60 10 – 50 33 – 15 50 – 120 Aluminum die castings 30 2 Aluminum alloy 17ST 56 34 26 39 100 Aluminum alloy 51ST 48 40 20 35 105 Copper, annealed 32 5 58 73 45 Copper, hard-drawn 68 60 4 55 100 Brasses, various 40 – 120 8 – 80 60 – 3 50 – 170 Phosphor bronze 40 – 130 55 – 5 50 – 200 Tobin bronze, rolled 63 41 40 52 120 Magnesium alloys, various 21 – 45 11 – 30 17 – 0.5 47 – 78 Monel 400, Ni-Cu alloy 79 30 48 75 125 Molybdenum, rolled 100 75 30 250 Silver, cast , annealed 18 8 54 27 Titanium 6 – 4 alloy, annealed 130 120 10 25 352 Ductile iron, grade 80-55-06 80 55 6 225 – 255 NOTE: Compressive strength of cast iron, 80,000 to 150,000 lb/in 2. Compressive yield strength of all metals, except those cold-worked ϭ tensile yield strength. Stress 1,000 lb/in 2 ϫ 6.894 ϭ stress, MN/m 2.men, resulting in what is known as the cup-and-cone fracture. Double to test temperature, test strain rate, and the characteristics of the tensilecup-and-cone and rosette fractures sometimes occur. Several types of machine employed.tensile fractures are shown in Fig. 5.1.3. The plastic behavior in a uniaxial tensile test can be represented as the Annealed or hot-rolled mild steels generally exhibit a yield point (see true stress-strain curve. The true stress is based on the instantaneousFig. 5.1.4). Here, in a constant strain-rate test, a large increment ofextension occurs under constant load at the elastic limit or at a stress justbelow the elastic limit. In the latter event the stress drops suddenly fromthe upper yield point to the lower yield point. Subsequent to the drop, theyield-point extension occurs at constant stress, followed by a rise to theUTS. Plastic ﬂow during the yield-point extension is discontinuous;Fig. 5.1.3. Typical metal fractures in tension.successive zones of plastic deformation, known as Luder’s bands orstretcher strains, appear until the entire specimen gage length has beenuniformly deformed at the end of the yield-point extension. This behav-ior causes a banded or stepped appearance on the metal surface. Theexact form of the stress-strain curve for this class of material is sensitive Fig. 5.1.4. Yielding of annealed steel.
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view.5-4 MECHANICAL PROPERTIES OF MATERIALScross section A, so that ϭ load/A. The instantaneous true strain incre- section. Methods of constructing the true stress-strain curve are de-ment is Ϫ dA/A, or dL/L prior to necking. Total true strain is scribed in the technical literature. In the range between initial ͵ ͩͪ A yielding and the neighborhood of the maximum load point the relation- dA A0 Ϫ ϭ ln ship between plastic strain p and true stress often approximates A0 A A ϭ kn por ln (L/L0 ) prior to necking. The true stress-strain curve or ﬂow curveobtained has the typical form shown in Fig. 5.1.5. In the part of the test where k is the strength coefﬁcient and n is the work-hardening exponent.subsequent to the maximum load point (UTS), when necking occurs, For a material which shows a yield point the relationship applies only tothe true strain of interest is that which occurs in an inﬁnitesimal length the rising part of the curve beyond the lower yield. It can be shown thatat the region of minimum cross section. True strain for this element can at the maximum load point the slope of the true stress-strain curvestill be expressed as ln (A0 /A), where A refers to the minimum cross equals the true stress, from which it can be deduced that for a material obeying the above exponential relationship between p and n, p ϭ n at the maximum load point. The exponent strongly inﬂuences the spread between YS and UTS on the engineering stress-strain curve. Values of n and k for some materials are shown in Table 5.1.2. A point on the ﬂow curve indentiﬁes the ﬂow stress corresponding to a certain strain, that is, the stress required to bring about this amount of plastic deformation. The concept of true strain is useful for accurately describing large amounts of plastic deformation. The linear strain deﬁnition (L Ϫ L 0 )/L 0 fails to correct for the continuously changing gage length, which leads to an increasing error as deformation proceeds. During extension of a specimen under tension, the change in the specimen cross-sectional area is related to the elongation by Poisson’s ratio , which is the ratio of strain in a transverse direction to that in the longitudinal direction. Values of for the elastic region are shown in Table 5.1.3. For plastic strain it is approximately 0.5. Table 5.1.2 Room-Temperature Plastic-Flow Constants for a Number of Metals k, 1,000 in 2 Material Condition (MN/m 2) n 0.40% C steel Quenched and tempered at 416 (2,860) 0.088 400°F (478K) 0.05% C steel Annealed and temper-rolled 72 (49.6) 0.235 2024 aluminum Precipitation-hardened 100 (689) 0.16 2024 aluminum Annealed 49 (338) 0.21 Copper Annealed 46.4 (319) 0.54 70 – 30 brass Annealed 130 (895) 0.49 SOURCE: Reproduced by permission from ‘‘Properties of Metals in Materials Engineering,’’Fig. 5.1.5. True stress-strain curve for 20°C annealed mild steel. ASM, 1949. Table 5.1.3 Elastic Constants of Metals (Mostly from tests of R. W. Vose) E G K Modulus of Modulus of elasticity rigidity (Young’s (shearing Bulk modulus). modulus). modulus. 1,000,000 1,000,000 1,000,000 Poisson’s Metal lb/in 2 lb/in2 lb/in 2 ratio Cast steel 28.5 11.3 20.2 0.265 Cold-rolled steel 29.5 11.5 23.1 0.287 Stainless steel 18 – 8 27.6 10.6 23.6 0.305 All other steels, including high-carbon, heat-treated 28.6 – 30.0 11.0 – 11.9 22.6 – 24.0 0.283 – 0.292 Cast iron 13.5 – 21.0 5.2 – 8.2 8.4 – 15.5 0.211 – 0.299 Malleable iron 23.6 9.3 17.2 0.271 Copper 15.6 5.8 17.9 0.355 Brass, 70 – 30 15.9 6.0 15.7 0.331 Cast brass 14.5 5.3 16.8 0.357 Tobin bronze 13.8 5.1 16.3 0.359 Phosphor bronze 15.9 5.9 17.8 0.350 Aluminum alloys, various 9.9 – 10.3 3.7 – 3.9 9.9 – 10.2 0.330 – 0.334 Monel metal 25.0 9.5 22.5 0.315 Inconel 31 11 0.27 – 0.38 Z-nickel 30 11 Ϯ 0.36 Beryllium copper 17 7 Ϯ 0.21 Elektron (magnesium alloy) 6.3 2.5 4.8 0.281 Titanium (99.0 Ti), annealed bar 15 – 16 6.5 0.34 Zirconium, crystal bar 11 – 14 Molybdenum, arc-cast 48 – 52
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. STRESS-STRAIN DIAGRAMS 5-5 The general effect of increased strain rate is to increase the resistance Tension or compression Bendingto plastic deformation and thus to raise the ﬂow curve. Decreasing test rtemperature also raises the ﬂow curve. The effect of strain rate is ex- I d IV ؉ /2pressed as strain-rate sensitivity m. Its value can be measured in the D 2r D dtension test if the strain rate is suddenly increased by a small increment d /2 ؉during the plastic extension. The ﬂow stress will then jump to a higher rvalue. The strain-rate sensitivity is the ratio of incremental changes of rlog and log II ؉ r ؉ ͩ ͪ V ␦ log D d mϭ D d ␦ log ؉ ؉ rFor most engineering materials at room temperature the strain rate sen- rsitivity is of the order of 0.01. The effect becomes more signiﬁcant at r III ؉elevated temperatures, with values ranging to 0.2 and sometimes higher. Compression Testing The compressive stress-strain curve is simi- D dlar to the tensile stress-strain curve up to the yield strength. Thereafter, ؉the progressively increasing specimen cross section causes the com- rpressive stress-strain curve to diverge from the tensile curve. Someductile metals will not fail in the compression test. Complex behavioroccurs when the direction of stressing is changed, because of the Baus- 3.4chinger effect, which can be described as follows: If a specimen is ﬁrstplastically strained in tension, its yield stress in compression is reduced Stress concentration factor, Kand vice versa. 3.0 Combined Stresses This refers to the situation in which stressesare present on each of the faces of a cubic element of the material. For a 2.6given cube orientation the applied stresses may include shear stresses Iover the cube faces as well as stresses normal to them. By a suitable IVrotation of axes the problem can be simpliﬁed: applied stresses on the 2.2 IInew cubic element are equivalent to three mutually orthogonal principalstresses 1 , 2 , 3 alone, each acting normal to a cube face. Combined 1.8stress behavior in the elastic range is described in Sec. 5.2, Mechanics IIIof Materials. V Prediction of the conditions under which plastic yielding will occur 1.4under combined stresses can be made with the help of several empirical Note; in all cases Dϭdϩ2rtheories. In the maximum-shear-stress theory the criterion for yielding is 1.0that yielding will occur when 0.01 0.1 0.2 1.0 1 Ϫ 3 ϭ ys r din which 1 and 3 are the largest and smallest principal stresses, re- Fig. 5.1.6. Flat plate with semicircular ﬁllets and grooves or with holes. I, II,spectively, and ys is the uniaxial tensile yield strength. This is the and III are in tension or compression; IV and V are in bending.simplest theory for predicting yielding under combined stresses. A moreaccurate prediction can be made by the distortion-energy theory, accord-ing to which the criterion is ؉ h r (1 Ϫ 2 )2 ϩ (2 Ϫ 3 ϩ (2 Ϫ )2 1)2 ϭ 2(ys )2 D d ؉r hStress-strain curves in the plastic region for combined stress loading canbe constructed. However, a particular stress state does not determine aunique strain value. The latter will depend on the stress-state path whichis followed. 3.4 02 Plane strain is a condition where strain is conﬁned to two dimensions. 0.There is generally stress in the third direction, but because of mechani- h ϭ d Stress concentration factor, Kcal constraints, strain in this dimension is prevented. Plane strain occurs 3.0 Semi-circle 05 0. 1in certain metalworking operations. It can also occur in the neighbor- grooves 0. (hϭr) 2hood of a crack tip in a tensile loaded member if the member is sufﬁ- 2.6 0.ciently thick. The material at the crack tip is then in triaxial tension,which condition promotes brittle fracture. On the other hand, ductility is 0. 5enhanced and fracture is suppressed by triaxial compression. 2.2 Blunt Sharp Stress Concentration In a structure or machine part having a notch grooves grooves 1or any abrupt change in cross section, the maximum stress will occur atthis location and will be greater than the stress calculated by elementary 1.8 2formulas based upon simpliﬁed assumptions as to the stress distribu-tion. The ratio of this maximum stress to the nominal stress (calculated 1.4by the elementary formulas) is the stress-concentration factor Kt . This isa constant for the particular geometry and is independent of the mate-rial, provided it is isotropic. The stress-concentration factor may be 1.0 0.4 1.0 1.5 2 3 4 5 6determined experimentally or, in some cases, theoretically from themathematical theory of elasticity. The factors shown in Figs. 5.1.6 to h Sharpness of groove,5.1.13 were determined from both photoelastic tests and the theory of relasticity. Stress concentration will cause failure of brittle materials if Fig. 5.1.7. Flat plate with grooves, in tension.
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view.5-6 MECHANICAL PROPERTIES OF MATERIALS ؉the concentrated stress is larger than the ultimate strength of the mate- r hrial. In ductile materials, concentrated stresses higher than the yield D dstrength will generally cause local plastic deformation and redistribu- r ؉ htion of stresses (rendering them more uniform). On the other hand, evenwith ductile materials areas of stress concentration are possible sites forfatigue if the component is cyclically loaded. 3.4 02 0. 5 d ϭ 0 .0 Stress concentration factor, K h 3.0 ؉ Dϭd ϩ 2h 1 0. r h 2.6 Full fillets D d (hϭr) 2 0. ؉ r h 2.2 Blunt Sharp fillets fillets 1.8 0.5 3.4 1 02 05 1.4 2 0. Stress concentration factor, K 0. 3.0 Dϭd ϩ 2h d ϭ ϭ h Full fillets 1 0. (hϭr) 1.0 et 2.6 0.4 1.0 1.5 2 3 4 5 6 fill 0.2 of h th Sharpness of fillet, p r De 2.2 Blunt Sharp 0.5 Fig. 5.1.10. Flat plate with ﬁllets, in bending. fillets fillets 1.8 1.0 2.0 1.4 1.0 0.4 1.0 1.5 2 3 4 5 6 h Sharpness of fillet, rFig. 5.1.8. Flat plate with ﬁllets, in tension. Fig. 5.1.11. Flat plate with angular notch, in tension or bending. ؉ r h ؉ d D r h D d ؉ r h 3.4 1 d ϭ 0. 3.4 5 0.4 0.0 0.1 h 3.0 d ϭ Stress concentration factor, K Dϭd ϩ 2h Stress concentration factor, K h 3.0 Semi circ. Semi-circle grooves hϭr 0.2 grooves 1 2.6 2.6 (hϭr) 2.2 Blunt Sharp 5 2.2 grooves grooves 0. Sharp grooves h 1.8 ϭ 0.04 1.8 1 d 4 2 1.4 1.4 10 1.0 1.0 0.4 1.0 1.5 2 3 4 5 6 0.5 1.0 1.5 2 3 4 5 6 8 10 15 20 h h Sharpness of groove, Sharpness of groove, r rFig. 5.1.9. Flat plate with grooves, in bending. Fig. 5.1.12. Grooved shaft in torsion.
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. FRACTURE AT LOW STRESSES 5-7 ؉ r h transition temperature of a material selected for a particular application D d is suitably matched to its intended use temperature. The DBT can be detected by plotting certain measurements from tensile or impact tests against temperature. Usually the transition to brittle behavior is com- plex, being neither fully ductile nor fully brittle. The range may extend over 200°F (110 K) interval. The nil-ductility temperature (NDT), deter- 3.4 h mined by the drop weight test (see ASTM Standards), is an important ϭ 0.05 d reference point in the transition range. When NDT for a particular steel Stress concentration factor, K 3.0 is known, temperature-stress combinations can be speciﬁed which de- Dϭd ϩ 2h ﬁne the limiting conditions under which catastrophic fracture can occur. 0.1 2 In the Charpy V-notch (CVN) impact test, a notched-bar specimen 0. 2.6 Full fillets (hϭr) (Fig. 5.1.26) is used which is loaded in bending (see ASTM Standards). Sharp fillets The energy absorbed from a swinging pendulum in fracturing the speci- 2.2 5 0. men is measured. The pendulum strikes the specimen at 16 to 19 ft Blunt (4.88 to 5.80 m)/s so that the specimen deformation associated with 1.8 1 fracture occurs at a rapid strain rate. This ensures a conservative mea- fillets sure of toughness, since in some materials, toughness is reduced by high 1.4 strain rates. A CVN impact energy vs. temperature curve is shown in Fig. 5.1.14, which also shows the transitions as given by percent brittle 1.0 fracture and by percent lateral expansion. The CVN energy has no 0.5 1.0 2 3 4 5 7 10 20 40 analytical signiﬁcance. The test is useful mainly as a guide to the frac- h ture behavior of a material for which an empirical correlation has been Sharpness of fillet, established between impact energy and some rigorous fracture criterion. r For a particular grade of steel the CVN curve can be correlated withFig. 5.1.13. Filleted shaft in torsion. NDT. (See ASME Boiler and Pressure Vessel Code.) Fracture Mechanics This analytical method is used for ultra-high-FRACTURE AT LOW STRESSES strength alloys, transition-temperature materials below the DBT tem-Materials under tension sometimes fail by rapid fracture at stresses perature, and some low-strength materials in heavy section thickness.much below their strength level as determined in tests on carefully Fracture mechanics theory deals with crack extension where plasticprepared specimens. These brittle, unstable, or catastrophic failures origi- effects are negligible or conﬁned to a small region around the crack tip.nate at preexisting stress-concentrating ﬂaws which may be inherent in The present discussion is concerned with a through-thickness crack in aa material. tension-loaded plate (Fig. 5.1.15) which is large enough so that the The transition-temperature approach is often used to ensure fracture- crack-tip stress ﬁeld is not affected by the plate edges. Fracture me-safe design in structural-grade steels. These materials exhibit a charac- chanics theory states that unstable crack extension occurs when theteristic temperature, known as the ductile brittle transition (DBT) tem- work required for an increment of crack extension, namely, surfaceperature, below which they are susceptible to brittle fracture. The tran- energy and energy consumed in local plastic deformation, is exceededsition-temperature approach to fracture-safe design ensures that the by the elastic-strain energy released at the crack tip. The elastic-stress Fig. 5.1.14. CVN transition curves. (Data from Westinghouse R & D Lab.)
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view.5-8 MECHANICAL PROPERTIES OF MATERIALSﬁeld surrounding one of the crack tips in Fig. 5.1.15 is characterized by Table 5.1.4 Room-Temperature K lc Values on High-Strengththe stress intensity KI, which has units of (lb √in) /in2 or (N√m) /m 2. It is Materials*a function of applied nominal stress , crack half-length a, and a geom- 0.2% YS, 1,000 in 2 K lc , 1,000 in 2etry factor Q: Material (MN/m 2) √in (MN m 1/2 /m 2) K 2 ϭ Q 2 a l (5.1.1) 18% Ni maraging steel 300 (2,060) 46 (50.7)for the situation of Fig. 5.1.15. For a particular material it is found that 18% Ni maraging steel 270 (1,850) 71 (78) 18% Ni maraging steel 198 (1,360) 87 (96)as KI is increased, a value Kc is reached at which unstable crack propa- Titanium 6-4 alloy 152 (1,022) 39 (43) Titanium 6-4 alloy 140 (960) 75 (82.5) Aluminum alloy 7075-T6 75 (516) 26 (28.6) Aluminum alloy 7075-T6 64 (440) 30 (33) * Determined at Westinghouse Research Laboratories. crack, and loadings (Paris and Sih, ‘‘Stress Analysis of Cracks,’’ STP- 381, ASTM, 1965). Failure occurs in all cases when Kt reaches KIc . Fracture mechanics also provides a framework for predicting the occur- rence of stress-corrosion cracking by using Eq. (5.1.2) with KIc replaced by KIscc , which is the material parameter denoting resistance to stress- corrosion-crack propagation in a particular medium. Two standard test specimens for KIc determination are speciﬁed in ASTM standards, which also detail specimen preparation and test pro- cedure. Recent developments in fracture mechanics permit treatment of crack propagation in the ductile regime. (See ‘‘Elastic-Plastic Frac- ture,’’ ASTM.)Fig. 5.1.15. Through-thickness crack geometry.gation occurs. Kc depends on plate thickness B, as shown in Fig. 5.1.16. FATIGUEIt attains a constant value when B is great enough to provide plane-strain Fatigue is generally understood as the gradual deterioration of a mate-conditions at the crack tip. The low plateau value of Kc is an important rial which is subjected to repeated loads. In fatigue testing, a specimenmaterial property known as the plane-strain critical stress intensity or is subjected to periodically varying constant-amplitude stresses byfracture toughness K Ic . Values for a number of materials are shown in means of mechanical or magnetic devices. The applied stresses mayTable 5.1.4. They are inﬂuenced strongly by processing and small alternate between equal positive and negative values, from zero to max-changes in composition, so that the values shown are not necessarily imum positive or negative values, or between unequal positive andtypical. KIc can be used in the critical form of Eq. (5.1.1): negative values. The most common loading is alternate tension and (KIc )2 ϭ Q 2acr (5.1.2) compression of equal numerical values obtained by rotating a smooth cylindrical specimen while under a bending load. A series of fatigueto predict failure stress when a maximum ﬂaw size in the material is tests are made on a number of specimens of the material at differentknown or to determine maximum allowable ﬂaw size when the stress is stress levels. The stress endured is then plotted against the number ofset. The predictions will be accurate so long as plate thickness B satis- cycles sustained. By choosing lower and lower stresses, a value may beﬁes the plane-strain criterion: B Ն 2.5(KIc/ys )2. They will be conserva- found which will not produce failure, regardless of the number of ap-tive if a plane-strain condition does not exist. A big advantage of the plied cycles. This stress value is called the fatigue limit. The diagram isfracture mechanics approach is that stress intensity can be calculated by called the stress-cycle diagram or S-N diagram. Instead of recording theequations analogous to (5.1.1) for a wide variety of geometries, types of data on cartesian coordinates, either stress is plotted vs. the logarithm of the number of cycles (Fig. 5.1.17) or both stress and cycles are plotted to logarithmic scales. Both diagrams show a relatively sharp bend in the curve near the fatigue limit for ferrous metals. The fatigue limit may be established for most steels between 2 and 10 million cycles. Nonferrous metals usually show no clearly deﬁned fatigue limit. The S-N curves in these cases indicate a continuous decrease in stress values to several hundred million cycles, and both the stress value and the number of cycles sustained should be reported. See Table 5.1.5. The mean stress (the average of the maximum and minimum stress values for a cycle) has a pronounced inﬂuence on the stress range (the algebraic difference between the maximum and minimum stress values). Several empirical formulas and graphical methods such as the ‘‘modiﬁed Goodman diagram’’ have been developed to show the inﬂu- ence of the mean stress on the stress range for failure. A simple but conservative approach (see Soderberg, Working Stresses, Jour. Appl. Mech., 2, Sept. 1935) is to plot the variable stress Sv (one-half the stress range) as ordinate vs. the mean stress Sm as abscissa (Fig. 5.1.18). At zero mean stress, the ordinate is the fatigue limit under completely reversed stress. Yielding will occur if the mean stress exceeds the yield stress So , and this establishes the extreme right-hand point of the dia- gram. A straight line is drawn between these two points. The coordi-Fig. 5.1.16. Dependence of K c and fracture appearance (in terms of percentage nates of any other point along this line are values of Sm and Sv whichof square fracture) on thickness of plate specimens. Based on data for aluminum may produce failure.7075-T6. (From Scrawly and Brown, STP-381, ASTM.) Surface defects, such as roughness or scratches, and notches or
Copyright (C) 1999 by The McGraw-Hill Companies, Inc. All rights reserved. Use of this product is subject to the terms of its License Agreement. Click here to view. FATIGUE 5-9 Accordingly, the pragmatic approach to arrive at a solution to a design problem often takes a conservative route and sets q ϭ 1. The exact material properties at play which are responsible for notch sensitivity are not clear. Further, notch sensitivity seems to be higher, and ordinary fatigue strength lower in large specimens, necessitating full-scale tests in many cases (see Peterson, Stress Concentration Phenomena in Fatigue of Fig. 5.1.18. Effect of mean stress on the variable stress for failure. Metals, Trans. ASME, 55, 1933, p. 157, and Buckwalter and Horger, Investigation of Fatigue Strength of Axles, Press Fits, Surface Rolling and Effect of Size, Trans. ASM, 25, Mar. 1937, p. 229). Corrosion andFig. 5.1.17. The S-N diagrams from fatigue tests. (1) 1.20% C steel, quenched galling (due to rubbing of mating surfaces) cause great reduction ofand drawn at 860°F (460°C); (2) alloy structural steel; (3) SAE 1050, quenched fatigue strengths, sometimes amounting to as much as 90 percent of theand drawn at 1,200°F (649°C); (4) SAE 4130, normalized and annealed; (5) ordi- original endurance limit. Although any corroding agent will promotenary structural steel; (6) Duralumin; (7) copper, annealed; (8) cast iron (reversedbending). severe corrosion fatigue, there is so much difference between the effects of ‘‘sea water’’ or ‘‘tap water’’ from different localities that numerical values are not quoted here.shoulders all reduce the fatigue strength of a part. With a notch of Overstressing specimens above the fatigue limit for periods shorterprescribed geometric form and known concentration factor, the reduc- than necessary to produce failure at that stress reduces the fatigue limittion in strength is appreciably less than would be called for by the in a subsequent test. Similarly, understressing below the fatigue limitconcentration factor itself, but the various metals differ widely in their may increase it. Shot peening, nitriding, and cold work usually improvesusceptibility to the effect of roughness and concentrations, or notch fatigue properties.sensitivity. No very good overall correlation exists between fatigue properties For a given material subjected to a prescribed state of stress and type and any other mechanical property of a material. The best correlation isof loading, notch sensitivity can be viewed as the ability of that material between the fatigue limit under completely reversed bending stress andto resist the concentration of stress incidental to the presence of a notch. the ordinary tensile strength. For many ferrous metals, the fatigue limitAlternately, notch sensitivity can be taken as a measure of the degree to is approximately 0.40 to 0.60 times the tensile strength if the latter iswhich the geometric stress concentration factor is reduced. An attempt below 200,000 lb/in2. Low-alloy high-yield-strength steels often showis made to rationalize notch sensitivity through the equation q ϭ (Kf Ϫ higher values than this. The fatigue limit for nonferrous metals is ap-1)/(K Ϫ 1), where q is the notch sensitivity, K is the geometric stress proximately to 0.20 to 0.50 times the tensile strength. The fatigue limitconcentration factor (from data similar to those in Figs. 5.1.5 to 5.1.13 in reversed shear is approximately 0.57 times that in reversed bending.and the like), and Kf is deﬁned as the ratio of the strength of unnotched In some very important engineering situations components are cycli-material to the strength of notched material. Ratio Kf is obtained from cally stressed into the plastic range. Examples are thermal strains result-laboratory tests, and K is deduced either theoretically or from laboratory ing from temperature oscillations and notched regions subjected to sec-tests, but both must reﬂect the same state of stress and type of loading. ondary stresses. Fatigue life in the plastic or ‘‘low-cycle’’ fatigue rangeThe value of q lies between 0 and 1, so that (1) if q ϭ 0, Kf ϭ 1 and the has been found to be a function of plastic strain, and low-cycle fatiguematerial is not notch-sensitive (soft metals such as copper, aluminum, testing is done with strain as the controlled variable rather than stress.and annealed low-strength steel); (2) if q ϭ 1, Kf ϭ K, the material is Fatigue life N and cyclic plastic strain p tend to follow the relationshipfully notch-sensitive and the full value of the geometric stress concen- N2 ϭ C ptration factor is not diminished (hard, high-strength steel). In practice, qwill lie somewhere between 0 and 1, but it may be hard to quantify. where C is a constant for a material when N Ͻ 105. (See Cofﬁn, A Study Table 5.1.5 Typical Approximate Fatigue Limits for Reversed Bending Tensile Fatigue Tensile Fatigue strength, limit , strength, limit , Metal 1,000 lb/in 2 1,000 lb/in 2 Metal 1,000 lb/in 2 1,000 lb/in 2 Cast iron 20 – 50 6 – 18 Copper 32 – 50 12 – 17 Malleable iron 50 24 Monel 70 – 120 20 – 50 Cast steel 60 – 80 24 – 32 Phosphor bronze 55 12 Armco iron 44 24 Tobin bronze, hard 65 21 Plain carbon steels 60 – 150 25 – 75 Cast aluminum alloys 18 – 40 6 – 11 SAE 6150, heat-treated 200 80 Wrought aluminum alloys 25 – 70 8 – 18 Nitralloy 125 80 Magnesium alloys 20 – 45 7 – 17 Brasses, various 25 – 75 7 – 20 Molybdenum, as cast 98 45 Zirconium crystal bar 52 16 – 18 Titanium (Ti-75A) 91 45 NOTE: Stress, 1,000 lb/in 2 ϫ 6.894 ϭ stress, MN/m 2.